Textile Fibers used in Eastern Aboriginal North America
Date: 2016-05-08T00:00:00+00:00
Keywords: Indian textile fabrics -- East (U.S.); Textile fibers

The Project Gutenberg eBook of Textile Fibers used in Eastern Aboriginal North America

This ebook is for the use of anyone anywhere in the United States and most other parts of the world at no cost and with almost no restrictions whatsoever. You may copy it, give it away or re-use it under the terms of the Project Gutenberg License included with this ebook or online at www.gutenberg.org. If you are not located in the United States, you will have to check the laws of the country where you are located before using this eBook.

Title: Textile Fibers used in Eastern Aboriginal North America

Author: A. C. Whitford

Release date: May 8, 2016 [eBook #52023]
Most recently updated: October 23, 2024

Language: English

Credits: Produced by Chris Curnow, Joseph Cooper, Sam W. and the
Online Distributed Proofreading Team at http://www.pgdp.net

*** START OF THE PROJECT GUTENBERG EBOOK TEXTILE FIBERS USED IN EASTERN ABORIGINAL NORTH AMERICA ***

ANTHROPOLOGICAL PAPERS
OF
THE AMERICAN MUSEUM OF NATURAL HISTORY

VOLUME XXXVIII, PART I

TEXTILE FIBERS USED IN EASTERN
ABORIGINAL NORTH AMERICA

By A. C. Whitford

By Order of the Trustees
of
THE AMERICAN MUSEUM OF NATURAL HISTORY
New York City
1941

THE AMERICAN MUSEUM OF NATURAL HISTORY

PUBLICATIONS IN ANTHROPOLOGY

In 1906 the present series of Anthropological Papers was authorized by the Trustees of the Museum to record the results of research conducted by the Department of Anthropology. The series comprises octavo volumes of about 350 pages each, issued in parts at irregular intervals. Previous to 1906 articles devoted to anthropological subjects appeared as occasional papers in the Bulletin and also in the Memoir series of the Museum. Of the Anthropological Papers 35 volumes have been completed. A complete list of these publications with prices will be furnished when requested. All communications should be addressed to the Librarian of the Museum.

The current volume is:—

VOLUME XXXVIII

I. Textile Fibers used in Eastern Aboriginal North America. By A. C. Whitford. Pp. 1-22. 1941. Price, $.25.

II. (In preparation.)

TEXTILE FIBERS USED IN EASTERN ABORIGINAL NORTH AMERICA

By A. C. Whitford

CONTENTS

| Page
INTRODUCTION | 5
MONOCOTYLEDONOUS SPECIES | 7
DIOCOTYLEDONOUS SPECIES | 9
OBJECTS FROM SPIRO MOUND, OKLAHOMA | 15
SUMMARY | 17
FIBER PLANTS AS IDENTIFIED | 17
TABLE OF IDENTIFICATIONS | 19

INTRODUCTION

The author of this paper has studied the vegetable fibers used in fabricating objects in the ethnological and archaeological collections from the Indian tribes of the Mississippi drainage and eastward, now in the American Museum. The first task was to identify them and view them against the background of existing textile knowledge. The present paper reports these identifications and comments upon fiber samples from collections in other museums.

The writing of this paper would have been impossible without the generous and whole-hearted coöperation of many institutions and individuals. This assistance has ranged from the furnishing of specimens for determination, to advice as to methods, classifications, and the supplying of modern material for comparison. For specimens of classified plants to be used in the comparative work thanks are due to The New York Botanical Garden in Bronx Park, the Botanical Departments of the University of Wisconsin, the University of Oklahoma, and the University of Georgia.

The standard histological microscopic methods were used for the determination of the fiber. Slides were made of both cross-sections and longitudinal sections and these were compared with previously prepared and classified modern material. When the specimen was too colored for microscopic examination it was bleached in a solution of Sodium perborate until clear enough for study. In charred material, when sufficient detail was preserved for identification the fiber sample was treated with Schultz Maceration solution, washed, dried, and fortified by saturating in a collodion solution. Occasionally, it was found necessary to stain the material and in this either Delafield’s Haematoxylon or Methylene Blue was used. In the differentiation of certain species, it was found necessary to make microscopic measurements of the length and width of the cells, but generally the shape, distribution, medullation, and other constant characters were sufficient for the identifications.

In the text and tables the following abbreviations are used for the names of the coöperating institutions:—

American Museum of Natural History | AMNH
Museum of the American Indian, Heye Foundation | MAIHF
Milwaukee Public Museum | MPM
McGill University Archaeological Museum | McGU
Ohio State Historical and Archaeological Museum | OSHAM
Peabody Museum, Harvard University | PMHU
Rochester Museum of Arts and Science | RMAS
University of Kentucky Museum | UKM
United States National Museum | USNM

MONOCOTYLEDONOUS SPECIES

The fibers from monocotyledonous plants, as identified, are listed here. Approximately five hundred objects were sampled, so the frequencies for the several species should be given that denominator.

ARECACEAE, Reichenb. (Palm Family)

The palmetto (Sabal palmetto, Walt.) seems to have been an article of commerce as it was used by the Winnebago and the Iroquois, north of its northern limit of distribution. It was also used by the Cherokee. The Winnebago used the fiber in the production of stiff cords for their bags. In three bags in the American Museum the stiff cords are made from this material (50-7531). For burden straps the Iroquois used this fiber to produce stiff strong cords which were covered with cotton or other soft fiber (AMNH 50.1-1954). The Cherokee used it in the manufacture of basketry (AMNH 50.1-2141).

BROMELIACEAE, J. St. Hil. (Pineapple Family)

This Florida moss (Tillandsia usneoides, L.) was found in specimens from the Southern States only. The Koasati and the people who built certain mounds in Florida used it frequently. A specimen in the United States National Museum from the Parish Mound, Number 2, in Florida, consisted of a bunch of loose material. The Koasati material is in the Museum of the American Indian, Heye Foundation, and is represented by fibers from a blanket and threads on a spindle (1-8551).

DRACAENACEAE, Link. (Yucca Family)

Yucca (Yucca arkansana, Trelease) was encountered in one specimen from the Arkansas Bluff culture in a bundle of loose fiber (MAIHF 11-7429).

Yucca (Yucca filamentosa, L.) was found once in a heavy cord made by the cave and shelter people of Ohio (OSHAM 332-42)

Nolina georgiana, Michx., was found in two specimens, a moccasin (OSHAM 332) and a bristle-like fiber from the Spiro Mound (2718-K, Trowbridge Collection). It is possible that this plant may have been used very frequently in objects from caves and rock-shelters. It was not always convenient, however, to examine complete objects so that some occurrences of its use may have been overlooked, especially since these people commonly mixed several fibers. In the specimen in question, for example (OSHAM 332), Nolina georgiana and Eryngium yuccaefolium were identified. Similar combinations of fibers from widely different plants have also been noted; frequently, as in the example cited, a local plant was mixed with one found at a great distance.

JUNIPERACEAE, Horan (Juniper Family)

Red cedar (Juniperus virginiana, L.) was encountered in only one specimen, a bag made by the Potawatomi Indians (AMNH 50.1-7096).

POACACEAE, R. Br. (Grass Family)

The grass family was the most commonly and widely used of any of the monocotyledonous families.

Big blue stem grass (Andropogon furcatus, Muhl.) was one of the major fibrous plants used by the cave and rock-shelter peoples of Ohio in the construction of coarsely woven articles, such as rope and moccasins. It was commonly used without preliminary treatment, but was simply twisted or braided into strands. The specimens examined were from the Ohio State Historical and Archaeological Museum. A typical example of the use of this fiber is in a woven moccasin (OSHAM 898-1).

Sweet grass (Hierochloe odorata, L.), to be distinguished from sweet vernal grass, was encountered only once in a bag made by the Michigan Ottawa Indians (MAIHF 19-7125).

Canebrake (Arundinaria tecta, Muhl.) was a common source of fiber for moccasins and rope. It seems to have been utilized by most of the prehistoric cave and rock-shelter peoples within its range (OSHAM 332-27).

TYPHACEAE, J. St. Hil. (Cat-tail Family)

The cat-tail (Typha latifolia, L.) was observed in a mat found in the caves of Tennessee (USNM 132252).

ZEA MAYS, L. (Indian Corn)

Indian corn occurred only once. This single occurrence has no real significance as to the frequency of its use, for all specimens in which it was obvious that corn was the material used were not sampled. The sample noted here was found in a knife made by the Micmac Indians (McGU H76). The material was a cornstalk which had been subjected to considerable pressure to force out the juice and pith to bring the hardy flinty layers into juxtaposition. It was then used as a wedge to fasten the knife handle. It was extremely hard and durable.

The above are the monocotyledons encountered in this survey, in all some twenty-four objects using this material. It should be noted that these materials are readily adaptable to use since they need very little preparation and are frequently used entire. Sometimes the fiber is removed from the surrounding materials by simply letting them ret. Yucca and Tillandsia are ordinarily used entire. The grasses were used as they were gathered, simply twisted or braided. Tillandsia is the only plant of this group which was used for the manufacture of fabrics as in the blanket above noted (p. 7). The specimen of cornstalk was an exception and its preparation was evidently for a specific purpose.

Palmetto fiber is especially adaptable. At the base of the leaves, where they join the main stem is a large mass of more or less loose or loosely interwoven fibrous material which needs only straightening to be ready for use.

DIOCOTYLEDONOUS SPECIES

ANONACEAE, D. C. (Custard-Apple Family)

The pawpaw (Asimina triloba, L.) seems to have been universally used by all the tribes who lived where it flourished. Its use was apparently limited only by its distribution, for it was encountered sixteen times in the prehistoric material examined from Kentucky, Arkansas, and Ohio, as well as in historic objects made by the Menomini and Wisconsin Potawatomi. In the University of Wisconsin Museum is a bunch of prepared fiber (16422) from the caves of Kentucky. This fiber was commonly used by the cave and rock-shelter peoples of Arkansas for cords, mats, rope, and in all coarsely woven materials. A woven mat from Bushwick Cave is a fair example (MAIHF 11-6243). The Ohio cave and rock-shelter dwellers used the pawpaw for coarse bags and fabrics, for example, in a split bark bag (OSHAM 332-22). In the Milwaukee Public Museum are two bags in which this fiber was identified, one, from the Menomini (4570) in which only the weft is of pawpaw, and another (23287) from the Wisconsin Potawatomi, entirely composed of it.

APOCYNACEAE, Lindl. (Dog-bane Family)

The genera Apocynum is represented by both the species indigenous to the territory surveyed, but as Indian hemp is one of them, it was rather surprising how infrequently they were encountered. Only ten examples of its use were found.

This plant (Apocynum androsaemifolium, L.) which is called dog-bane is so similar in appearance and properties that it might well have been and was used indiscriminately with Indian hemp (Apocynum cannabinum, L.). The species was found three times in material examined. Its use by the Nanticoke in the manufacture of fish nets is demonstrated by a net (50.2-600) in the American Museum. A burden strap (50-7221) made from this fiber by the Iroquois is also in the Museum collections.

Apocynum cannabinum L., the so-called Indian hemp, was found seven times and of these is represented four times in the archaeological cave and rock-shelter materials examined. The Museum of the American Indian, Heye Foundation, has a bundle of prepared fibers (11-7384) found at Allards Bluff, Arkansas. A dark colored piece of fabric, attributed to the Hopewell culture of Ohio, made in part from this material (957) is in the collections of the Ohio State Historical and Archaeological Museum. Another piece of cloth (1200) in the same museum is an Adena culture example of the use of this fiber. The Museum of the American Indian, Heye Foundation, has a Sauk and Fox bag (2-4694) made from this fiber. In the American Museum a fish net (50.2-601) made by the Nanticoke and an Iroquois burden strap (50-7401) complete the catalogue of objects in which this fiber occurs. In many of the older specimens examined, the fiber was crudely prepared before twisting, but in the more recent Indian material it is well broken down and fine, so as to make small counts and even threads or cords.

ASCLEPIADACEAE, Lindl. (Milkweed Family)

The milkweed family is represented by four species of Asclepias, namely, tuberosa, pulchra, incarnata, and syriaca. These fibers were used in the manufacture of fine threads and cords. In both archaeological and recent Indian material the fibers were well prepared before use. In the archaeological objects it is possible that the fibers were collected in the spring, after retting by the weather; in any event, they all show that they have been freed to a large extent of their cementitious materials and epidermis.

The highland milkweed (Asclepias tuberosa, L.) was encountered twelve times from all parts of its geographical range. The cave dwellers of Arkansas used it, as is exemplified by a bundle of knotted fibers in the Museum of the American Indian, Heye Foundation (11-6179). In the Peabody Museum of Harvard University is some textile material which accompanied a knife found in an Ohio mound (28328). The protohistoric Indians of Massachusetts used the fiber to manufacture textiles as may be seen in a piece of plain cloth (A4127) and in a specimen of twined cloth (A5478) in the same museum. The Iroquois Indians employed it to make fine threads for stringing wampum belts as is shown by one (M1905) in the Archaeological Museum of McGill University. As stated above, all this material was broken down to make comparatively fine, smooth threads and cords.

The species, Asclepias pulchra, Ehrh., or swamp milkweed, is closely related to A. incarnata, L. It was found in ten specimens examined, but from only two states, Ohio and Kentucky. In the University of Kentucky Museum is a rope (Bh-15/V4), made of this fiber. In the Ohio State Historical and Archaeological Museum are specimens of fabrics made from it which are attributed to the Hopewell culture. One of these, a piece of cloth wrapped around a copper plate (283), also contains Urtica gracilis.

The milkweed (Asclepias incarnata, L.) was noted four times in Ohio archaeological objects. In the Ohio State Historical and Archaeological Museum is a two-strand rope (899-20), one strand of which is made from this fiber. This is a typical cave and rock-shelter sample. Wrapped around a Hopewell culture copper plate in the same museum is a piece of fabric containing five different fibers, among them Asclepias incarnata (957).

The species Asclepias syriaca, L., seems to be the most widely distributed geographically of any used by the Indians surveyed in this paper. It was found seventeen times in material from all sections and many tribes.

In this Museum were observed the following objects in which this fiber was used in whole or in combination with other fiber: a Sauk and Fox bag (50-4886); a Delaware drum string (50.1-1609); a Delaware burden strap (50-7244); a Matchapunga fish net (50.1-9911); and a cord used, for wrapping on a spear (50.1-7475), Micmac. In the Museum of the American Indian, Heye Foundation, is a Kickapoo ball of string (2-5294) made of this fiber. In an Iroquois wampum belt (M1913) in the Archaeological Museum of McGill University, the beads are strung on cords made from this fiber. An Iroquois burden strap (AE 360) in the Rochester Museum of Arts and Sciences is composed of this fiber. Fiber of this species was also used by the prehistoric cave and rock-shelter people of Ohio as is shown by a fish net (OSHAM 332-23) in the Ohio State Historical and Archaeological Museum.

BETULACEAE, Agardh. (Birch Family)

The paper birch (Betula papyrifera, Marsh.) was encountered in one specimen (AMNH 50.2-1792). The bark was untreated, simply twisted into a cord. In a specimen of Iroquois horsehair embroidery (McGU H49) the bark had received no preliminary treatment, but was used in the raw state.

CANNABINACEAE, Lindl. (Hop Family)

This introduced plant, hemp (Cannabis sativa, L.), was found in four specimens, evidently made in post-Columbian times as the plant is not indigenous to the Western Hemisphere, but was introduced by the colonists at a very early date. It was found in a bag (MPM 28116) made by the Wisconsin Potawatomi Indians. A bowstring on an Algonkin bow (AMNH 50.2-4221A) is made from this fiber as are also portions of an Oneida burden strap (AMNH 50.1-1800).

DAPHNACEAE (Mezereon Family)

This moose or leatherwood fiber (Dirca palustris, L.) was encountered eleven times in as widely separated states as Arkansas and Wisconsin. It was used both in the raw state, as strips twisted into cord, and as treated fiber in finer cords and threads. A prehistoric mat made by the inhabitants of Bushwick Cave, Arkansas, is composed of this material (MAIHF 19-4635). Cloth of the Adena culture made, in part, from this bast fiber (1200) is in the Ohio State Historical and Archaeological Museum. In the Milwaukee Public Museum is a Wisconsin Potawatomi bag (23447) in which the weft is nicely prepared fiber from this plant. In the collections of this Museum is a Winnebago bag (50-784D) woven with two kinds of cord; light colored cord of Dirca palustris and dark colored cord of Tilia americana.

JUGLANDACEAE, Lindl. (Walnut Family)

The bast from the black walnut (Juglans nigra, L.) was encountered twice in burden straps from the Iroquois (Museum of the American Indian, Heye Foundation). These fibers had apparently been previously treated, both chemically and mechanically. They were probably boiled in ashes, pounded, and then straightened so as to make them usable in twisting cord and thread. One such specimen in the above Museum carries the catalogue number 16-5208.

LINACEAE, Dumort. (Flax Family)

Common flax (Linum usitatissimum, L.) is another example of introduced fibers used by the Indians in post-Columbian times. The fiber was probably secured in trade. It was found in five specimens made by the Winnebago, Potawatomi, Michigan, Ottawa, and Delaware Indians. In the Milwaukee Public Museum is a bag (14619), made by the Winnebago and composed entirely of flax cords. In a Delaware burden strap (50-7191) in this Museum the fine cords are linen, but the coarse cords are milkweed, Asclepias syriaca. In the Archaeological Museum of McGill University is a wampum belt (M5932), the beads of which are strung on a commercial linen thread.

MALVACEAE, Neck. (Mallow Family)

As was to be expected, cotton (Gossypium herbaceum, L.) became the most commonly and universally used of any of the fibers after it was introduced east of the Mississippi River. No specimen was encountered in the prehistoric material, but after its introduction and sale by traders it was the most commonly used fiber. It does not seem advisable to discuss these uses in detail, suffice it to say that it served all purposes for which string and thread are utilized.

SALICACEAE, Lindl. (Willow Family)

Black willow (Salix nigra, Marsh.). This species of black willow was used by the Menomini, Winnebago, Michigan Ottawa, and Ojibway Indians in the manufacture of bags, pouches, fish nets, and cord. A Menomini bag (MAIHF 8-1136) and a similar Winnebago bag (AMNH 50.1-903) contain black willow fiber. A Micmac fish spear (AMNH 50-4754) is wrapped with black willow twine. In the preparation of black willow fiber the bark was obviously stripped from the tree. Then the inner white bast tissue was removed and boiled in wood ashes; finally, this bast was pounded and rubbed to remove all the cementitious materials and loosen the fibers so they could be arranged more or less parallel to each other for twisting or spinning. In none of the specimens examined were crude strips of the inner bark used without preliminary treatment.

TILIACEAE, Juss. (Basswood Family)

The bast layer from the basswood (Tilia americana, L.) seems to have been the fiber most commonly and universally used by the Eastern Indians, for it was encountered fifty-two times, in all areas from which specimens were obtained, with the exception of the extreme south. It was utilized for nearly all purposes, from the manufacture of bags to textiles. In the Milwaukee Public Museum is a Menomini bag (4586) made from the Tilia bast, carefully and thoroughly prepared to remove the gums and render the fibers parallel and capable of being spun into good yarn. A Potawatomi bag in this Museum (50.1-7091) is made from the same material. In the Museum of the American Indian, Heye Foundation, is a bag made by the Sauk and Fox (2-4966). In the Peabody Museum of Harvard University is a twilled woven garment (A5479B) made by the protohistoric Indians of Massachusetts. An Iroquois burden strap (AE 2963) in the Rochester Museum of Arts and Sciences is woven of threads from prepared fibers from this tree. In the Ohio State Historical and Archaeological Museum is a prehistoric fabric (957) containing Tilia and three other species of fiber. Hopewell mound and rock-shelter specimens in the same museum show the use of Tilia.

The above gives a general picture of basswood fiber usage. It was found in an untreated state, merely cut into strips, as well as thoroughly treated and spun into comparatively fine threads.

ULMACEAE, Mirbel. (Elm Family)

The slippery elm (Ulmus fulva, Michx.) was found three times. Once, in a burden strap made by the Iroquois Indians (AMNH 50-6680) in which the fibers had received some preliminary treatment to soften them and remove much of the natural gum. Two other specimens, both rather coarsely woven fabrics from mounds of the Hopewell culture (OSHAM 283 and 125) were in the Ohio State Historical and Archaeological Museum.

The American elm (Ulmus americana, L.) was encountered only once in an Iroquois burden strap (MAIHF 19-4550). The fiber had received some preliminary treatment and differed decidedly from Ulmus fulva in the shape of the cells, in cross-section, and the residual amount of amorphous material.

UMBELLIFERAE

The eryngium (Eryngium yuccaefolium, Michx.) was commonly used by the prehistoric tribes of the area in which it occurs. It was found fifty-five times in material from the caves and rock-shelters of Arkansas, Kentucky, Tennessee, and Ohio. Its parallel veined long leaves lend themselves to all uses as readily as the yuccas of the south and west. It is easily shredded or it can be used entire with equal facility. The stem contains a very strong bast fiber which was also utilized. It does not seem to have been utilized by the historic Indians, as it was not encountered outside of the above cultures. Whatever, if any, treatment it received before usage was very slight and consisted apparently of shredding, with no chemical treatment, as no fine threads or cords were found. A sandal from the Kentucky cave culture is made from this plant by utilizing the leaf, as in the Southwest. A cord from a reed mat found in the Tennessee caves (USNM 132252) is made from this material. The cord was used for tying reeds (Typha latifolia, L.) together. The Museum of the American Indian, Heye Foundation, contains many specimens taken from the caves and rock-shelters of Arkansas. Among these is a bag (11-7315) from Allards Bluff, made of this material.

This plant was frequently encountered in collections from the Hopewell and the rock-shelter cultures of Ohio, in the State Museum at Columbus; as, braided work (957), and cloth from a burial (854). These objects are believed to be typical, but the same plant was used in all classes of cordage and textiles found in collections representing these cultures.

URTICACEAE, Reichenb. (Nettle Family)

The nettle family is represented by three genera, Boehmeria, Urtica, and Laportea. Specimens of these three were encountered forty-eight times, so it seems to have been one of the most important families as a source of fibrous materials. The tissues were, almost without exception, treated before use.

The stingless nettle (Boehmeria cylindrica, L.) was used by practically all the Indian tribes covered by this survey. It was invariably more or less treated, with the possible exception of some twisted strands from the Bushwick Cave of Arkansas (MAIHF 19-4632). This cord appears to have been made by simply peeling the bark from the plant and twisting it. The Delaware used the same fiber in a wampum string (AMNH 50.1-1579), also in a burden strap (AMNH 50.1-1592). A Cherokee string used in a feather charm occurs in the collection of the Museum of the American Indian, Heye Foundation. The handle of a Micmac curved knife (McGU H76) is fastened to the blade by wrapping with cord of this fiber. In the same museum there are two Iroquois wampum belts in which the strings for the beads are made from Boehmeria fiber. In the American Museum are two specimens of cord, one on a Micmac fish spear (50.1-7475) and the other the string to an Ojibway bow (50-6874A).

It is evident that raw Boehmeria fiber, properly treated, produces especially fine, soft, and strong material. It is easily distinguished from the fibers of the other members of the family by its smaller size, the shape of the cells, and their distribution when seen in cross-section. Both the Urtica and Laportea fibers are coarser and the ratio of length to width of the fiber is much greater. The lumen in all three is longer one way than the other, but is much more open in Boehmeria cylindrica than the other species.

The slender nettle (Urtica gracilis, Ait.) seems to have been a favorite source for all peoples from prehistoric to modern Indians. Its use extended from New England to Wisconsin. It was usually processed before use, except among some of the prehistoric peoples where it was merely twisted into cord. A bag from the caves of Tennessee (USNM 132255) is made from this fiber which has had some preliminary treatment. A modern Sauk and Fox bag (MAIHF 2-7911) shows complete preliminary processing. Some string in the Peabody Museum of Harvard University (A4109), is made from this plant; this is protohistoric material. The Hopewell culture of Ohio is represented by twelve specimens using this fiber, all of which show some preliminary treatment. A sample of cloth from a copper plate is representative (OSHAM 283). The cave and rock-shelter cultures of Ohio are represented, but here the fiber seems to have received little, if any, preliminary treatment prior to use (OSHAM 332-42).

The woods nettle (Laportea canadensis, L.) was most widely used of all of the Urticaceae, both before and after treatment. It was used by the Sauk and Fox for bags, after it had received thorough treatment. In the Milwaukee Public Museum is a bag (30260) made of this material, thoroughly treated before being twisted into fine cord. A string used for tying a spear point to a shaft is in the Ojibway collection of the American Museum (50-4748). The Iroquois used it to make burden straps (MAIHF 19-8895). Braided cloth from prehistoric Kentucky is represented by a specimen (56795) in the Peabody Museum of Harvard University. The cave culture of Tennessee is represented in the United States National Museum by a shirt (132254) made from this fiber. The Hopewell culture of Ohio is well represented by fabrics in the Ohio State Historical and Archaeological Museum (957, is an example). The cave and rock-shelter culture of the same state employed this fiber to make twined cords as is exemplified by a cord (OSHAM 332-34). The cave and rock-shelter cultures of Arkansas used it for the manufacture of twisted cords as may be seen in a specimen (19-4630) in the Museum of the American Indian, Heye Foundation.

OBJECTS FROM SPIRO MOUND, OKLAHOMA

The well-known Spiro Mound, clearly prehistoric, furnished some examples of basketry, matting, cord, and cloth. The samples were sent to the writer by Mr. H. M. Trowbridge, Bethel, Kansas.

2716-C | Twisted fibers covered with feathers | Arundinaria tecta
2716-H | Twisted fibers covered with feathers | Asimina triloba
2717-C | Twisted fibers covered with feathers | Asimina triloba
2717-G | Woody material with feathers attached | Asimina triloba
2717-I&E | Twisted fiber mass | Asimina triloba
2718-E | Twisted fiber mass | Asimina triloba
2718-K | Bristle-like vegetable fiber | Nolina georgiana
2719-J | Twisted vegetable fiber | Asimina triloba
2721-A | Mat | Arundinaria tecta
2721-S | Fragment of basketry | Arundinaria tecta
2722-D | Twisted fiber | Arundinaria tecta
2722-I | Twisted fiber covered with feathers | Arundinaria tecta
2724-A | Twisted fiber covered with feathers | Arundinaria tecta
2724-K | Fawn colored string | Arundinaria tecta
2731 | Mat | Arundinaria tecta
2782 | Copper stained rope | Asimina triloba
2781 | Charred basket | Arundinaria tecta
2783 | Fibers adhering to copper sheet | Arundinaria tecta

A comparison of materials in prehistoric collections reveals an excess of animal materials in the artifacts from Spiro Mound. One gets the impression that in Spiro textiles strings of vegetable fiber are usually surfaced with hair or other animal materials to increase the softness of the product. This may account for the almost exclusive use of canebrake and pawpaw, both relatively coarse fibers used without preliminary treatment. A striking contrast is between the slipshod way of making string and the highly precise fine techniques of covering it with hair and feathers.

SUMMARY

This survey makes no pretension of being complete, but it is an adequate sampling of the fibers utilized by the Eastern Indians and illustrates their resourcefulness in exploiting the raw materials at hand. It is noticeable that they used a great variety of plants and that one of the determining properties or qualifications was the local abundance of a plant. There seems to have been a tendency to use the monocotyledonous plants and the bast from the trees for coarser work and the diocotyledonous herbaceous plants for the manufacture of finer cords and threads.

Several general points of interest are apparent from the comparative study of these prehistoric and historic plant materials.

1. The plant fibers used by the prehistoric people were rarely if ever treated before utilization, while among the modern Indians a high degree of skill has been attained in the preparation of the fibers before spinning.

2. There seems to have been some commercial interchange between the Northern and the Southern tribes, both in historic and prehistoric times. The occurrence of palmetto fibers in modern Mohawk and Potawatomi collections and the use of Nolina by the cave and rock-shelter people of Ohio, shows commerce.

3. It seems that most, if not all, of the materials utilized were wild plants for there was no discoverable evidence of the cultivation of these plants. Such evidence would be far from obvious since cultivation does not seem to improve the fibers in textile plants.

4. Among the prehistoric peoples the purposeful mixing of fibers was the rule. This is especially notable in the collections from Ohio and Arkansas. These mixtures of fibers occur both in the same strand and in the two-ply cords. It is not apparent why the fibers from different plants were mixed, but the combinations seem intentional, as nettle and milkweed, blue stem grass and pawpaw, nettle and yucca, basswood and nettle, and pawpaw and yucca. Yet, such intentional mixtures were rarely encountered in the historic collections examined.

5. It is apparent that the prehistoric peoples used such fibers as were adapted to their immediate purpose without previous treatment. They were stripped from the plant and twisted at once. This seems to account for the dominance of monocotyledonous fibers in prehistoric collections. The historic Indians, on the other hand, used a greater variety of species of fiber plants because they were able to prepare them properly before using. The determining factors seem to have been strength, fineness of fiber, and abundance of supply.

All the above observations are consistent with the assumption of a steady advance in textile skill and knowledge from prehistoric time to the present.

FIBER PLANTS AS IDENTIFIED

Andropogon furcatus | Blue stem grass
Apocynum cannabinum, androsaemifolium | Indian hemp
Arundinaria tecta | Canebrake
Asclepias syriaca, tuberosa, pulchra, incarnata | Milkweed
Asimina triloba | Pawpaw
Betula papyrifera | Paper birch
Boehmeria cylindrica | Stingless nettle
Cannabis sativa | Hemp
Dirca palustris | Moosewood
Eryngium yuccaefolium |
Gossypium herbaceum | Cotton
Hierochloe odorata | Sweet grass
Juglans nigra | Black walnut
Juniperus virginiana | Red cedar
Laportea canadensis | Woods nettle
Linum usitatissimum | Flax
Nolina georgiana | Yucca
Sabal palmetto | Palmetto
Salix nigra | Black willow
Tilia americana | Basswood
Tillandsia usneoides | Florida moss
Typha latifolia | Cat-tail
Ulmus americana, fulva | Elm
Urtica gracilis | Slender nettle
Yucca arkansana, filamentosa | Yucca
Zea mays | Indian corn

TABLE OF IDENTIFICATIONS

Selected objects in museum collections to show the range and frequencies in the use of vegetable fibers, including geographical and chronological distributions.

The objects from the Ohio State Historical and Archaeological Museum are all prehistoric. In other museums prehistoric objects are marked with an asterisk (*).

American Museum of Natural History

Number | Object | Fiber
ALGONKIN
50.2-4221A | String from bow | Cannabis sativa
CHEROKEE
50.1-2141 | Basket | Coarse material, Sabal palmetto; fine material, cotton
50.1-9911 | Fish net | Asclepias syriaca
50.1-1901a | Moccasin | Corchorus capsularis, jute
DELAWARE
50-7191 | Burden strap | Fine cord, Linum usitatissimum; coarse cord, Asclepias syriaca
50.1-1592 | Burden strap | Boehmeria cylindrica
50-7244 | Burden strap | Asclepias syriaca
50-7243 | Burden strap | Asclepias syriaca
50-7203 | Ceremonial wampum | Tilia americana
50.1-1609 | Drum string | Asclepias syriaca
50.1-1621 | Rope | Tilia americana
50.1-1579 | Wampum string | Boehmeria cylindrica
IROQUOIS

50-6683

Burden strap

Light-colored string, Asclepias syriaca; dark-colored loose material, Sabal palmetto; dark-colored string, Tilia americana

50-6682 | Burden strap | Light-colored string, cotton; dark-colored string, Tilia americana
50-6680 | Burden strap | Ulmus fulva
50-6681 | Burden strap | Brown cord, cotton; light-colored material, Laportea canadensis; dark-colored material, Tilia americana
50-7221 | Burden strap | Apocynum androsaemifolium
50-7401 | Burden strap | Apocynum cannabinum
50.1-1800 | Burden strap | Cannabis sativa, hemp
50.1-1954 | Pack frame | Cotton, palmetto, and Tilia americana
MATCHAPUNGA
50.1-9911 | Fishnet | Asclepias syriaca
MENOMINI
50-9885 | Reed mat | Tilia americana
50.1-5880 | Bag | Cotton
50-9864 | Bag | Soft string, cotton; stiff cord, Tilia americana
50-9871 | Bag | Cotton
50-9873 | Bag | Cotton
50-9867 | Bag | Cotton
50-9872 | Bag | Cotton
50-9866 | Bag | Cotton
50-4798 | Bag | Cotton
50-9877 | Bag | Tilia americana
50.1-6862 | Bag | Tilia americana
50-9880 | Bag | Tilia americana
MICMAC
50.1-7475 | Fish spear | Dark stiff cord, Boehmeria cylindrica; gray cord, Asclepias syriaca
NANTICOKE
50.2-601 | Netting | Apocynum cannabinum
50.2-600 | Netting | Apocynum androsaemifolium
OJIBWAY
50-6874a | Bow | Boehmeria cylindrica
50-4754 | Fish net | Salix nigra
50-4749 | Fish hook wrapping | Salix nigra
50-4748 | Spear wrapping | Laportea canadensis
50-5690 | Woven bag | Cotton
50-4600 | Woven bag | Yellow threads, animal; gray threads, cotton
PAMUNKEY
50.1-9907 | Net | Cotton
50.1-9906 | Net | Cotton
50.1-9897 | Net | Cotton
POTAWATOMI
50.1-7098 | Bag | Tilia americana
50.1-6895 | Bag | White cord, cotton; dark loose fiber, Tilia americana
50.1-7091 | Bag | Tilia americana
50.1-6899 | Bag | Cotton
50.1-7096 | Bag | Cotton and cedar
50.1-6897 | Bag | Cotton and animal
50.1-7090 | Bag | Cotton
50.1-7095 | Bag | Cotton and animal
SAUK AND FOX
50.1-2169 | Bag | Tilia americana
50-4886 | Bag | Light and dark, Asclepias syriaca
50-3558 | Bag | Cotton
50-3550 | Bag | Cotton
50-2219 | Bag | Cotton
50.1-2168 | Bag | Cotton
50-4885 | Bag | Animal
50-3570 | Fiber for making bags | Laportea canadensis
50-2204 | String | Asclepias tuberosa
WINNEBAGO
50.1-903 | Bag | Red fiber, Salix nigra
50-7573 | Bag | Blue and red yarn, animal; gray, cotton; stiff cord, Tilia americana
50-7531 | Bag | Soft cord, cotton; hard cord and loose fiber, Sabal palmetto
50-7572 | Bag | White cord, cotton; loose fibers, Sabal palmetto
50.1-906 | Bag | Tilia americana
50.1-907 | Bag | Cotton and animal (wool?)
50-7533 | Bag | Cotton and animal
50-7759 | Bag | Cotton and animal
50-784D | Bag | Light-colored cord, Dirca palustris; dark-colored cord, Tilia americana
50-7532 | Bag | Light cord, Tilia americana; dark-colored cord, Salix nigra
50-7574 | Bag | Stiff cords, Tilia americana; soft cords, Dirca palustris
50.1-904 | Bag | Cords, cotton; loose fibers, Tilia americana
50-7760 | Bag | Cotton and animal
50-7763 | Bag | Cotton and animal
50-7843 | Bag | Cotton and animal
50.2-8024 | Bag | Cotton
50-7762 | Bag | Cotton
50.1-905 | Bag | Soft cord, cotton; hard cord, Sabal palmetto

Museum of the American Indian, Heye Foundation

Number | Object | Fiber | Tribe or Location
2-4694 | Bag | Apocynum cannabinum | Sauk and Fox
2-4966 | Bag | Tilia americana | Sauk and Fox
2-7911 | Bag | Urtica gracilis | Sauk and Fox
8-1136 | Bag | Salix nigra | Menomini
11-6232* | Bag | Eryngium yuccaefolium | Arkansas
11-7315* | Bag | Eryngium yuccaefolium | Arkansas
19-7125 | Bag | Hierochloe odorata |
16-5208 | Burden strap | Juglans nigra | Mohawk
19-4550 | Burden strap | Ulmus americana | Iroquois
2-5294 | Cord | Asclepias syriaca | Kickapoo
19-4632* | Cord | Boehmeria cylindrica | Arkansas
11-6179* | Cord | Asclepias tuberosa | Arkansas
11-7384* | Cord | Apocynum cannabinum | Arkansas
11-7429* | Cord | Yucca arkansana and Asimina triloba | Arkansas
1-8551 | Cord | Tillandsia usneoides | Koasati
11-8575* | Cord | Asimina triloba | Arkansas
19-4630* | Cord | Laportea canadensis | Arkansas
1-8672 | Saddle blanket | Tillandsia usneoides | Koasati
19-8146 | Cord on a kettle | Apocynum androsaemifolium | Iroquois
11-6243* | Mat | Asimina triloba | Arkansas
19-4635* | Mat | Dirca palustris | Arkansas

Ohio State Historical and Archaeological Museum

Number | Object | Fiber
332-22 | Bag | Asimina triloba
332-34 | Cord | Eryngium yuccaefolium; Laportea canadensis
332-42 | Cord | Yucca filamentosa
898-1 | Cord | Andropogon furcatus
899-20 | Cord | Asclepias incarnata
7 | Fabric | Asclepias pulchra
125 | Fabric | Ulmus fulva
283 | Fabric | Asclepias pulchra; Urtica gracilis; Ulmus fulva
332 | Fabric | Andropogon furcatus; Asimina triloba; Arundinaria tecta
854 | Fabric | Eryngium yuccaefolium
957 | Fabric | Eryngium yuccaefolium; Tilia americana; Asclepias incarnata; Apocynum cannabinum; Laportea canadensis
1200 | Fabric | Dirca palustris; Apocynum cannabinum
1175 | Mat | Arundinaria tecta
332 | Moccasin | Nolina georgiana
332-27 | Moccasin | Arundinaria tecta
332-23 | Net | Asclepias syriaca

Milwaukee Public Museum

Number | Object | Fiber
4570 | Bag | Asimina triloba
4586 | Bag | Tilia americana
14619 | Bag | Linum usitatissimum
23287 | Bag | Asimina triloba
23447 | Bag | Dirca palustris
28116 | Bag | Cannabis sativa
30260 | Bag | Laportea canadensis
33076 | Fabric | Urtica gracilis

University of Kentucky Museum

Number | Object | Fiber
Le-5/V2* | Netting | Asclepias pulchra
Bh-15/V4 | Netting | Asclepias pulchra

University of Wisconsin Museum

Number | Object | Fiber
16422* | Fiber | Asimina triloba

Rochester Museum of Arts and Sciences

Number | Object | Fiber
AE2963 | Burden strap | Tilia americana
AE 360 | Burden strap | Asclepias syriaca

McGill University Archaeological Museum

Number | Object | Fiber
H76 | Cord | Zea mays; Boehmeria cylindrica
M1911 | Cord | Tilia americana
11083 | Cord | Asclepias tuberosa
M1905 | Wampum belt | Asclepias tuberosa
M1908 | Wampum belt | Asclepias tuberosa
M1912 | Wampum belt | Boehmeria cylindrica
M1913 | Wampum belt | Asclepias syriaca
M5932 | Wampum belt | Linum usitatissimum

United States National Museum

Number | Object | Fiber
132255* | Bag | Urtica gracilis
132254* | Fabric | Laportea canadensis
132252* | Mat (reeds) | Typha latifolia
132252* | Cord | Eryngium yuccaefolium
132253* | Fabric | Laportea canadensis

Peabody Museum, Harvard University

Number | Object | Fiber
A4109 | Cord | Urtica gracilis
A4127* | Fabric | Asclepias tuberosa
A5478 | Fabric | Asclepias tuberosa
A5479B | Fabric | Tilia americana
28328* | Fabric | Asclepias tuberosa
28390* | Fabric | Eryngium yuccaefolium
56795 | Fabric | Laportea canadensis
8232 | Moccasin | Eryngium yuccaefolium

Transcriber’s Note

Variant spelling is preserved as printed.

Minor punctuation errors have been repaired.

On page 17, the common name for Eryngium yuccaefolium is omitted from the table ‘Fiber Plants as Identified.’ It is typically identified as button eryngo, button snake-root or rattlesnake master. The omission in the table is preserved as printed.

On page 21, there is nothing in the ‘Tribe or location’ column for the bag, 19-7125, in the table ‘Museum of the American Indian, Heye Foundation.’

On page 22, there were no column labels on the tables from ‘University of Kentucky Museum’ onwards. For ease of reference, the transcriber has added column labels.

*** END OF THE PROJECT GUTENBERG EBOOK TEXTILE FIBERS USED IN EASTERN ABORIGINAL NORTH AMERICA ***

Updated editions will replace the previous one—the old editions will be renamed.

Creating the works from print editions not protected by U.S. copyright law means that no one owns a United States copyright in these works, so the Foundation (and you!) can copy and distribute it in the United States without permission and without paying copyright royalties. Special rules, set forth in the General Terms of Use part of this license, apply to copying and distributing Project Gutenberg™ electronic works to protect the PROJECT GUTENBERG™ concept and trademark. Project Gutenberg is a registered trademark, and may not be used if you charge for an eBook, except by following the terms of the trademark license, including paying royalties for use of the Project Gutenberg trademark. If you do not charge anything for copies of this eBook, complying with the trademark license is very easy. You may use this eBook for nearly any purpose such as creation of derivative works, reports, performances and research. Project Gutenberg eBooks may be modified and printed and given away—you may do practically ANYTHING in the United States with eBooks not protected by U.S. copyright law. Redistribution is subject to the trademark license, especially commercial redistribution.

START: FULL LICENSE

THE FULL PROJECT GUTENBERG LICENSE

PLEASE READ THIS BEFORE YOU DISTRIBUTE OR USE THIS WORK

To protect the Project Gutenberg™ mission of promoting the free distribution of electronic works, by using or distributing this work (or any other work associated in any way with the phrase “Project Gutenberg”), you agree to comply with all the terms of the Full Project Gutenberg™ License available with this file or online at www.gutenberg.org/license.

Section 1. General Terms of Use and Redistributing Project Gutenberg™ electronic works

1.A. By reading or using any part of this Project Gutenberg™ electronic work, you indicate that you have read, understand, agree to and accept all the terms of this license and intellectual property (trademark/copyright) agreement. If you do not agree to abide by all the terms of this agreement, you must cease using and return or destroy all copies of Project Gutenberg™ electronic works in your possession. If you paid a fee for obtaining a copy of or access to a Project Gutenberg™ electronic work and you do not agree to be bound by the terms of this agreement, you may obtain a refund from the person or entity to whom you paid the fee as set forth in paragraph 1.E.8.

1.B. “Project Gutenberg” is a registered trademark. It may only be used on or associated in any way with an electronic work by people who agree to be bound by the terms of this agreement. There are a few things that you can do with most Project Gutenberg™ electronic works even without complying with the full terms of this agreement. See paragraph 1.C below. There are a lot of things you can do with Project Gutenberg™ electronic works if you follow the terms of this agreement and help preserve free future access to Project Gutenberg™ electronic works. See paragraph 1.E below.

1.C. The Project Gutenberg Literary Archive Foundation (“the Foundation” or PGLAF), owns a compilation copyright in the collection of Project Gutenberg™ electronic works. Nearly all the individual works in the collection are in the public domain in the United States. If an individual work is unprotected by copyright law in the United States and you are located in the United States, we do not claim a right to prevent you from copying, distributing, performing, displaying or creating derivative works based on the work as long as all references to Project Gutenberg are removed. Of course, we hope that you will support the Project Gutenberg™ mission of promoting free access to electronic works by freely sharing Project Gutenberg™ works in compliance with the terms of this agreement for keeping the Project Gutenberg™ name associated with the work. You can easily comply with the terms of this agreement by keeping this work in the same format with its attached full Project Gutenberg™ License when you share it without charge with others.

1.D. The copyright laws of the place where you are located also govern what you can do with this work. Copyright laws in most countries are in a constant state of change. If you are outside the United States, check the laws of your country in addition to the terms of this agreement before downloading, copying, displaying, performing, distributing or creating derivative works based on this work or any other Project Gutenberg™ work. The Foundation makes no representations concerning the copyright status of any work in any country other than the United States.

1.E. Unless you have removed all references to Project Gutenberg:

1.E.1. The following sentence, with active links to, or other immediate access to, the full Project Gutenberg™ License must appear prominently whenever any copy of a Project Gutenberg™ work (any work on which the phrase “Project Gutenberg” appears, or with which the phrase “Project Gutenberg” is associated) is accessed, displayed, performed, viewed, copied or distributed:

This eBook is for the use of anyone anywhere in the United States and most other parts of the world at no cost and with almost no restrictions whatsoever. You may copy it, give it away or re-use it under the terms of the Project Gutenberg License included with this eBook or online at www.gutenberg.org. If you are not located in the United States, you will have to check the laws of the country where you are located before using this eBook.

1.E.2. If an individual Project Gutenberg™ electronic work is derived from texts not protected by U.S. copyright law (does not contain a notice indicating that it is posted with permission of the copyright holder), the work can be copied and distributed to anyone in the United States without paying any fees or charges. If you are redistributing or providing access to a work with the phrase “Project Gutenberg” associated with or appearing on the work, you must comply either with the requirements of paragraphs 1.E.1 through 1.E.7 or obtain permission for the use of the work and the Project Gutenberg™ trademark as set forth in paragraphs 1.E.8 or 1.E.9.

1.E.3. If an individual Project Gutenberg™ electronic work is posted with the permission of the copyright holder, your use and distribution must comply with both paragraphs 1.E.1 through 1.E.7 and any additional terms imposed by the copyright holder. Additional terms will be linked to the Project Gutenberg™ License for all works posted with the permission of the copyright holder found at the beginning of this work.

1.E.4. Do not unlink or detach or remove the full Project Gutenberg™ License terms from this work, or any files containing a part of this work or any other work associated with Project Gutenberg™.

1.E.5. Do not copy, display, perform, distribute or redistribute this electronic work, or any part of this electronic work, without prominently displaying the sentence set forth in paragraph 1.E.1 with active links or immediate access to the full terms of the Project Gutenberg™ License.

1.E.6. You may convert to and distribute this work in any binary, compressed, marked up, nonproprietary or proprietary form, including any word processing or hypertext form. However, if you provide access to or distribute copies of a Project Gutenberg™ work in a format other than “Plain Vanilla ASCII” or other format used in the official version posted on the official Project Gutenberg™ website (www.gutenberg.org), you must, at no additional cost, fee or expense to the user, provide a copy, a means of exporting a copy, or a means of obtaining a copy upon request, of the work in its original “Plain Vanilla ASCII” or other form. Any alternate format must include the full Project Gutenberg™ License as specified in paragraph 1.E.1.

1.E.7. Do not charge a fee for access to, viewing, displaying, performing, copying or distributing any Project Gutenberg™ works unless you comply with paragraph 1.E.8 or 1.E.9.

1.E.8. You may charge a reasonable fee for copies of or providing access to or distributing Project Gutenberg™ electronic works provided that:

- • You pay a royalty fee of 20% of the gross profits you derive from the use of Project Gutenberg™ works calculated using the method you already use to calculate your applicable taxes. The fee is owed to the owner of the Project Gutenberg™ trademark, but he has agreed to donate royalties under this paragraph to the Project Gutenberg Literary Archive Foundation. Royalty payments must be paid within 60 days following each date on which you prepare (or are legally required to prepare) your periodic tax returns. Royalty payments should be clearly marked as such and sent to the Project Gutenberg Literary Archive Foundation at the address specified in Section 4, “Information about donations to the Project Gutenberg Literary Archive Foundation.”

- • You provide a full refund of any money paid by a user who notifies you in writing (or by e-mail) within 30 days of receipt that s/he does not agree to the terms of the full Project Gutenberg™ License. You must require such a user to return or destroy all copies of the works possessed in a physical medium and discontinue all use of and all access to other copies of Project Gutenberg™ works.

- • You provide, in accordance with paragraph 1.F.3, a full refund of any money paid for a work or a replacement copy, if a defect in the electronic work is discovered and reported to you within 90 days of receipt of the work.

- • You comply with all other terms of this agreement for free distribution of Project Gutenberg™ works.

1.E.9. If you wish to charge a fee or distribute a Project Gutenberg™ electronic work or group of works on different terms than are set forth in this agreement, you must obtain permission in writing from the Project Gutenberg Literary Archive Foundation, the manager of the Project Gutenberg™ trademark. Contact the Foundation as set forth in Section 3 below.

1.F.

1.F.1. Project Gutenberg volunteers and employees expend considerable effort to identify, do copyright research on, transcribe and proofread works not protected by U.S. copyright law in creating the Project Gutenberg™ collection. Despite these efforts, Project Gutenberg™ electronic works, and the medium on which they may be stored, may contain “Defects,” such as, but not limited to, incomplete, inaccurate or corrupt data, transcription errors, a copyright or other intellectual property infringement, a defective or damaged disk or other medium, a computer virus, or computer codes that damage or cannot be read by your equipment.

1.F.2. LIMITED WARRANTY, DISCLAIMER OF DAMAGES - Except for the “Right of Replacement or Refund” described in paragraph 1.F.3, the Project Gutenberg Literary Archive Foundation, the owner of the Project Gutenberg™ trademark, and any other party distributing a Project Gutenberg™ electronic work under this agreement, disclaim all liability to you for damages, costs and expenses, including legal fees. YOU AGREE THAT YOU HAVE NO REMEDIES FOR NEGLIGENCE, STRICT LIABILITY, BREACH OF WARRANTY OR BREACH OF CONTRACT EXCEPT THOSE PROVIDED IN PARAGRAPH 1.F.3. YOU AGREE THAT THE FOUNDATION, THE TRADEMARK OWNER, AND ANY DISTRIBUTOR UNDER THIS AGREEMENT WILL NOT BE LIABLE TO YOU FOR ACTUAL, DIRECT, INDIRECT, CONSEQUENTIAL, PUNITIVE OR INCIDENTAL DAMAGES EVEN IF YOU GIVE NOTICE OF THE POSSIBILITY OF SUCH DAMAGE.

1.F.3. LIMITED RIGHT OF REPLACEMENT OR REFUND - If you discover a defect in this electronic work within 90 days of receiving it, you can receive a refund of the money (if any) you paid for it by sending a written explanation to the person you received the work from. If you received the work on a physical medium, you must return the medium with your written explanation. The person or entity that provided you with the defective work may elect to provide a replacement copy in lieu of a refund. If you received the work electronically, the person or entity providing it to you may choose to give you a second opportunity to receive the work electronically in lieu of a refund. If the second copy is also defective, you may demand a refund in writing without further opportunities to fix the problem.

1.F.4. Except for the limited right of replacement or refund set forth in paragraph 1.F.3, this work is provided to you ‘AS-IS’, WITH NO OTHER WARRANTIES OF ANY KIND, EXPRESS OR IMPLIED, INCLUDING BUT NOT LIMITED TO WARRANTIES OF MERCHANTABILITY OR FITNESS FOR ANY PURPOSE.

1.F.5. Some states do not allow disclaimers of certain implied warranties or the exclusion or limitation of certain types of damages. If any disclaimer or limitation set forth in this agreement violates the law of the state applicable to this agreement, the agreement shall be interpreted to make the maximum disclaimer or limitation permitted by the applicable state law. The invalidity or unenforceability of any provision of this agreement shall not void the remaining provisions.

1.F.6. INDEMNITY - You agree to indemnify and hold the Foundation, the trademark owner, any agent or employee of the Foundation, anyone providing copies of Project Gutenberg™ electronic works in accordance with this agreement, and any volunteers associated with the production, promotion and distribution of Project Gutenberg™ electronic works, harmless from all liability, costs and expenses, including legal fees, that arise directly or indirectly from any of the following which you do or cause to occur: (a) distribution of this or any Project Gutenberg™ work, (b) alteration, modification, or additions or deletions to any Project Gutenberg™ work, and (c) any Defect you cause.

Section 2. Information about the Mission of Project Gutenberg™

Project Gutenberg™ is synonymous with the free distribution of electronic works in formats readable by the widest variety of computers including obsolete, old, middle-aged and new computers. It exists because of the efforts of hundreds of volunteers and donations from people in all walks of life.

Volunteers and financial support to provide volunteers with the assistance they need are critical to reaching Project Gutenberg™’s goals and ensuring that the Project Gutenberg™ collection will remain freely available for generations to come. In 2001, the Project Gutenberg Literary Archive Foundation was created to provide a secure and permanent future for Project Gutenberg™ and future generations. To learn more about the Project Gutenberg Literary Archive Foundation and how your efforts and donations can help, see Sections 3 and 4 and the Foundation information page at www.gutenberg.org.

Section 3. Information about the Project Gutenberg Literary Archive Foundation

The Project Gutenberg Literary Archive Foundation is a non-profit 501(c)(3) educational corporation organized under the laws of the state of Mississippi and granted tax exempt status by the Internal Revenue Service. The Foundation’s EIN or federal tax identification number is 64-6221541. Contributions to the Project Gutenberg Literary Archive Foundation are tax deductible to the full extent permitted by U.S. federal laws and your state’s laws.

The Foundation’s business office is located at 809 North 1500 West, Salt Lake City, UT 84116, (801) 596-1887. Email contact links and up to date contact information can be found at the Foundation’s website and official page at www.gutenberg.org/contact

Section 4. Information about Donations to the Project Gutenberg Literary Archive Foundation

Project Gutenberg™ depends upon and cannot survive without widespread public support and donations to carry out its mission of increasing the number of public domain and licensed works that can be freely distributed in machine-readable form accessible by the widest array of equipment including outdated equipment. Many small donations ($1 to $5,000) are particularly important to maintaining tax exempt status with the IRS.

The Foundation is committed to complying with the laws regulating charities and charitable donations in all 50 states of the United States. Compliance requirements are not uniform and it takes a considerable effort, much paperwork and many fees to meet and keep up with these requirements. We do not solicit donations in locations where we have not received written confirmation of compliance. To SEND DONATIONS or determine the status of compliance for any particular state visit www.gutenberg.org/donate.

While we cannot and do not solicit contributions from states where we have not met the solicitation requirements, we know of no prohibition against accepting unsolicited donations from donors in such states who approach us with offers to donate.

International donations are gratefully accepted, but we cannot make any statements concerning tax treatment of donations received from outside the United States. U.S. laws alone swamp our small staff.

Please check the Project Gutenberg web pages for current donation methods and addresses. Donations are accepted in a number of other ways including checks, online payments and credit card donations. To donate, please visit: www.gutenberg.org/donate.

Section 5. General Information About Project Gutenberg™ electronic works

Professor Michael S. Hart was the originator of the Project Gutenberg™ concept of a library of electronic works that could be freely shared with anyone. For forty years, he produced and distributed Project Gutenberg™ eBooks with only a loose network of volunteer support.

Project Gutenberg™ eBooks are often created from several printed editions, all of which are confirmed as not protected by copyright in the U.S. unless a copyright notice is included. Thus, we do not necessarily keep eBooks in compliance with any particular paper edition.

Most people start at our website which has the main PG search facility: www.gutenberg.org.

This website includes information about Project Gutenberg™, including how to make donations to the Project Gutenberg Literary Archive Foundation, how to help produce our new eBooks, and how to subscribe to our email newsletter to hear about new eBooks.

Table of Contents

- TEXTILE FIBERS USED IN EASTERN ABORIGINAL NORTH AMERICA

- CONTENTS

- INTRODUCTION

- MONOCOTYLEDONOUS SPECIES

- ARECACEAE, Reichenb. (Palm Family)

- BROMELIACEAE, J. St. Hil. (Pineapple Family)

- DRACAENACEAE, Link. (Yucca Family)
- JUNIPERACEAE, Horan (Juniper Family)
- POACACEAE, R. Br. (Grass Family)
- TYPHACEAE, J. St. Hil. (Cat-tail Family)
- ZEA MAYS, L. (Indian Corn)

- DIOCOTYLEDONOUS SPECIES

- ANONACEAE, D. C. (Custard-Apple Family)
- APOCYNACEAE, Lindl. (Dog-bane Family)
- ASCLEPIADACEAE, Lindl. (Milkweed Family)
- BETULACEAE, Agardh. (Birch Family)
- CANNABINACEAE, Lindl. (Hop Family)
- DAPHNACEAE (Mezereon Family)
- JUGLANDACEAE, Lindl. (Walnut Family)
- LINACEAE, Dumort. (Flax Family)
- MALVACEAE, Neck. (Mallow Family)
- SALICACEAE, Lindl. (Willow Family)
- TILIACEAE, Juss. (Basswood Family)
- ULMACEAE, Mirbel. (Elm Family)
- UMBELLIFERAE
- URTICACEAE, Reichenb. (Nettle Family)

- OBJECTS FROM SPIRO MOUND, OKLAHOMA
- SUMMARY
- FIBER PLANTS AS IDENTIFIED

- TABLE OF IDENTIFICATIONS

- American Museum of Natural History

- Museum of the American Indian, Heye Foundation

- Ohio State Historical and Archaeological Museum

- Milwaukee Public Museum
- University of Kentucky Museum
- University of Wisconsin Museum
- Rochester Museum of Arts and Sciences
- McGill University Archaeological Museum
- United States National Museum
- Peabody Museum, Harvard University

- THE FULL PROJECT GUTENBERG LICENSE